- Mobile Flash Butt Welding
TABLE OF CONTENT MobileFlash Butt Welding Uses of Mobile Flash Butt Welding Various Options in Mobile Flash Butt Welding Staff Requirement for Mobile Flash Butt welding Mobile Flash Butt Welding Procedure Pre Welding Checks Actual Welding Procedure Testing of Welds Precautions in Mobile Flash Butt Welding Mobile Flash Butt Welding Mobile Flash Butt Welding is a Rail cum Road Machine.Mobile Flash Butt Welding Plant is a four wheeled mobilevehicle, which can travel on roads with rubberised wheelsand on rails with metal wheels in which the following arefitted: Welding Equipment Welding Parameter Recorder Separate units for Grinding & USFD Testing Equipment Mobile Flash Butt Welding Plant moving on track Unloading the welding Equipment from the vehicleModel AMS60 Made Schlatter Unloading the welding Equipment from the vehicleModel K-920 Holland Made Uses of Mobile Flash Butt Welding The basic use of the Mobile Flash Butt Welding is to use theflash butt welding technique in field which otherwisecannot be done using the static plant. The Mobile Flash ButtWelding is preferable as the welds have much better fatiguestrength and performance as compared to the AT weldingotherwise used. It is basically used for the followingpurposes: In construction works for converting free rails or 3 railpanels (which is the maximum possible to be laid in newlines due to transportation constraints) to LWR. In open Line for Through Weld renewal to replace weldswhich have completed their life. Various Options in Mobile Flash Butt Welding FIXED SITE DEPOTS MOBILE DEPOTS MOBILE FBW PLANT The different options have their own advantages & disadvantages: SL No FIXED SITE DEPOTS MOBILE DEPOTS MOBILE FBW PLANT 1 Panels can be made at At convenient locations, the Plant moves and reaches one point only. depots can be setup and theevery point of welding. Transportation has to panels will require to be be done.transported from this location only. 2 Time for welding is Time for welding is min but Time for welding less. Time forsetting up of plants takesmaximum as plant to be transportation of some time at each location. setup for each weld. No panels maximum. Transportation of panelstransportation of panels. takes lesser time. 3 Suitable for smallerSuitable for construction Suitable for construction lengths of track whereprojects if the welding workprojects if the track one set up can serveto form panels is to be done in possession can be given for the entire stretch in parallel with the other works.the plant to work. Work construction as well as In open line, suitable for TWRwill commence only after open line.and the plant can be setupthe rails are laid on near any level crossing orcompleted formation. approachable location. Staff Requirement for Mobile Flash Butt welding The Welding team may consist of one Supervisor and twowelders. The educational qualification of the Supervisorshould be minimum Diploma in Mechanical / ElectricalEngg. or B.Sc and that of welder should be minimum Class Xor equivalent pass. Zonal Railways should ensure periodictraining of welders on Mobile Flash Butt Welding Plant. Thecompetency certificate of welder of Mobile Flash ButtWelding Plant is issued by the Zonal Railways. The Supervisor and Welder of the Plant should haveacquaintance in knowledge of the following. Welding parameters and its influence on quality of weldingand heat affected zone Suitability of rails for welding Preparation of rails to be welded including prestraightening of rails Procedure of welding of rails Record of welds Post weld straightening of rails Finishing of joints Marking of joints Testing of welds Precautions to avoid defects in rail joints Mobile Flash Butt Welding Procedure There are three basic mechanisms in the machine: CLAMPING MECHANISM FORGING MECHANISM TRANSFORMER The Schematic representation of a Mobile Flash ButtWelding unit is as follows: Basic Principle of Flash Butt Welding The basic principle is that heat is generated by electricresistance method at the ends of two rails to be weldedwhich were firmly clamped into the jaws of the weldingmachine. Both the jaws of the machine are movable and assuch, the gap between the two rail ends can be adjusted. Pre Welding Checks Preparation of rails before welding: In constructionwork, the free rails transported to the site of work areplaced over the uniformly spaced sleepers over the ballastbed on the formation, without clipping them with thesleepers, with their ends are butt each other. In open line, 7sleepers on either side of the weld are to be opened out forthe welding process. Aligning the rails in construction project Aligning the rails in construction project Straightening & Cleaning of rail ends Straightening of rails : The rails ends are required to bestraightened with the help of hydraulic rams before weldingso as to get good alignment of the welded rail . Cleaning of rail ends: The rail ends shall be cleaned usinggrinders to get clean surface. Photo showing rail cleaned by grinding Inspection of Rail ends A thorough inspection of rail ends shall be carried out andthe deviation of vertical and horizontal misalignmentshould be within the tolerable limits as given below: Individual welded ends may have a maximum difference inheight of 1.2 mm as in case of second hand rails. If the rail wear is not equal, the grouping of railsso that maximum difference of height doesnot exceed 1.2 mm shall be done as shown in figure Welding of second hand rails Second hand rails within the following limit of tolerancecan also be welded using Mobile Flash Butt Welding: Rail New Rail Second Hand Rail 60Kg 172.00 mm164 mm 52Kg 156.00 mm150 mm 90R142.88mm 139 mm Rail New Rail Second Hand Rail 60Kg 72.00 mm 66 mm 52Kg 67.00 mm 61 mm 90R66.68mm61 mmThe tolerance on the end bends in the vertical plane should be (+) 0.7mm and (-) 0.0mmon a straight edge of 1.5 m. Tolerances for rail in vertical planeThe tolerance on the end bends in the horizontal plane should be (+) or (-)0.7mm on a straight edge of 1.5 m. Tolerances specified for rail endsThe dimensions of the head width of rail should be checked and should be lessthan 0.5 mm deviation Rail head checking gauge for 60Kg rail Tolerances for rail endsThe rail ends shall be cut vertically and these shall be as per tolerances given below: Actual Welding Procedure Clamping the rail ends: The mobile flash butt welding machine is loweredfrom the vehicle and the rail ends which are close together are clamped. TheThe rail ends are then brought together so that almost touch each other tocreate the flash. The longitudinal and vertical alignment of the rail is correctedby suitable adjustments of the machine. The rail ends being clamped by the welding machine The rail ends being clamped by the welding machine The rail ends clamped and welding process about tobegin Close up view of the rail ends clamped by thewelding machine Setting up the flash The rails are brought towards each other till the flash starts.The flash will lead to heat generation which will soften thesteel. The electric energy is switched on and thereby allowingand electric current of about 5 volts and 35,000 Amperes topass between interfaces of two rails. Lot of flashing takesplace and considerable heat is generated by the passage ofelectric current between the rail ends. The rail ends are moved to and fro automatically by themachine till the temperature rises to the fusion limits in therange of 1000 C to 1500 C. Starting up the flash Flashing for welding Flashing for welding (another view) Applying force The rail ends are then hydraulically pressed so that thesoftened rail ends fuse together to form weld. At this juncture, the rail ends are pressed together with anupset pressure of about 37 T. The final flashing takes place joining the two rail endstogether. The welding is so regulated that any steel thatmight have been oxidized during the heating process getscompletely squeezed out. Applying hydraulic force Stripping the weld As soon the rails are welded, they are made to pass througha stripping Unit where all the extra metal called upsets ischipped off. The removal of metal by stripping is so goodthat except the head no other portion require any finishing. Stripping the weld Weld completedThe average time taken for welding a joint is about 6 minutes per joint and No.of joints that can be welded is about 50 to 55 joints per 8 hrs shift. Grinding rail endsThe rail table and gauge face of the joints thus welded, arefinally ground to correct rail profile, by means of a trolleygrinder for the rail table and by pneumatic grinders for otherportions. Post straightening & Ultrasonic TestingPost straightening: The rails are post straightened mechanically to removehorizontal and vertical kinks so as to give perfect alignment in both directions.Ultrasonic Testing: The welded rails are then ultrasonically tested with normal 70and 45 probes. Weld numbering and identificationEach weld shall be given a number so as to identify the weld, welder andcorrelation can be established between the field weld and the weld record. Testing of Welds Weld recorder: The machine has a weld recorder which measures and stores the weldingparameters. The results are stored in machine and can be retrieved later on also. Print out canalso be obtained of the welding parameters which can be used as permanent record. Thefollowing parameters are recorded (figures in brackets are standard values): Pre Flash Time (47 sec) Flash Time (95 sec) Boost Time (07 sec) Up set Time (1.8 sec) Forge Time (2 sec) Current Set (190 280 Amps) Forge Force (38 65 Tons) Up set Rail Use (12.7 mm) Welding parameters will depend on section and metallurgy of rail to be welded. These are,normally, specified by the manufacturer of the plant. Before adoption, the welding parametersshall be got approved from RDSO. RDSO shall consider parameters suggested by themanufacturer while fixing the parameters. Standardized for Flash Butt Welding Plant Zonal Railways / Owner of Mobile Flash Butt Welding Plant arerequired to get the welding parameters standardized for their FlashButt Welding Plant for different rail chemistry and rail section inconsultation with RDSO, Lucknow before regular operation of the plant.RDSO will standardize welding parameters for a particular machine,make and model. These standardized parameters shall be circulated toZonal Railways and shall be applicable for same type of machineworking on other Zonal Railways also. For Mobile Flash Butt WeldingPlant of particular make for which standardized parameters exist,sample testing will be carried out either at RDSO or at the nearest FlashButt Welding Plant (having the testing facilities) in presence of RDFSOofficial to check the compliance of machine. For all Mobile Flash Butt Welding Plants, QAP will be approved by RDSObefore plant is put to regular operation. The welding parameters shouldbe available with welder of the plant and displayed at appropriate pointon the plant. Following tests shall be conducted on the welds: Testing of Flash Butt Welded Joints Hardness Test: Brinnel hardness test shall be conducted on the test weldsample before conducting transverse load test. The hardness value in HAZ shallnot vary from the hardness of the parent rail by more than + 20 HB. Resultsshall be maintained as per proforma given in Annexure VI C. Extent of heat affected zone (max value in mm) Head 38 mm Web 39 mm Foot 36 mm The results of tests shall be maintained. VALUES OF MINIMUM BREAKING LOAD AND DEFLECTION IN TRANSVERSELOAD TEST: Testing Frequency of Flash Butt Welded Joints Sample joints for first 1000 Joints welded by a Mobile Flash butt welding plant will be tested at a frequency of 1in 100 joints and subsequently at a frequency of 1 in 500 joints. As Per RDSO Manual Rail section Span Min.Min.Frequency of testing BreakingDeflection Load (tones)At StationaryRDSO ManualAs per Mobile & plant FBWP centre(mm)60 Kg. (UIC) NHH 1.25m115 301 IN 5001 in 10060 Kg (UIC) Cr. Mn. 1.25m110 121 IN 5001 in 100Alloy steel60 Kg. UIC (90 UTS)1m150 201 in 1000 1 in 10052 kg. 90 UTS1m100 151 in 1000 1 in 10060 Kg (UIC) MM (721m135 301 in 1000 1 in 100UTS)52 Kg MM (72 UTS)1m100 301 in 1000 1 in 10090R MM (72 UTS)1m 80 301 in 1000 1 in 10075R MM (72 UTS)1m 70 301 in 1000 1 in 10060R MM (72 UTS)1m 60 251 in 1000 1 in 100 Testing of Flash Butt Welded Joints Macro Examination test: One test joint for every 1000joints welded in case of mobile flash butt welding plantshall be subjected to macro examination. 150 mm length ofrail with weld at centre shall be cut and the sample shall besectioned in vertical, longitudinal directions through theweld. One of the sections shall be etched with 5 10%Nitric acid and also subjected to magna flux test to ensurefreedom fro cracks, lack of fusion or oxide inclusion. Extentof heat affected zone shall be measured for head, foot andweb of the rail. These values should not be more than thevalues achieved during standardization of weldingparameters of the particular rail section and chemistry ofparticular make of FBW Plant. Results shall be maintainedas per proforma. Precautions in Mobile Flash Butt Welding End squareness of rail faces must be ensured. Better weld strength with minimum value andmerely parallel shape of heat affecting zone can be achieved using perfect matching of rail ends. Secondary out put of current should be sufficient enough to achieve complete fusion of buttingfaces. Butting stroke should be sufficient for complete coalescence (not less than 12 mm) Throughout Uniform and smooth auto trimming of the squeezed out metal and completegrinding using profile grinder. Minimum and nearly parallel heat affected zone of the joint should be achieved. Facilities for auto recording of weld parameters including final butting pressure shall beavailable. When weld is carried out in situ, minimum 20 minutes time after trimming is required to passthe first train through the weld with proper packing and support below the joint. Track should be levelled. Excess butting pressure leads to high joints. These are strictly prohibited and shall be closelymonitored by trained departmental staff. To avoid buckling of track, the continuous welding is prohibited in skeleton track and a gapshould be left at every 500 m interval which will be used for destressing. (In new line works) Night welding and welding during rainy session to be avoided as far as possible for obtainingbetter results. Target should not be fixed more than 40 joints per working day in order to keep sufficient timegap before moving allowing the machine over the newly welded joints.(In new line works) Computer printout has to be obtained for each weld just after the execution in order to rectifythe variations in various parameters as recommended before commencement of the next joint..